data_global
#===============================================================================
_publ_contact_author		  'Masato Kakihana'
_publ_contact_author_phone        '+81/22/217-5649'
_publ_contact_author_fax          '+81/22/217-5649'
_publ_contact_author_email        'kakihana@tagen.tohoku.ac.jp'
_publ_requested_journal           'Dalton Transactions'
_publ_section_title
;
Crystal Structures and Luminescence Properties of Eu2+-activated new 
NaBa0.5Ca0.5PO4 and Na3Ba2Ca(PO4)3
;

 _publ_author_address
;       
*********
Institute of Multidisciplinary Research for Advanced Materials
Tohoku University
2-1-1 Katahira, Aoba-ku, Sendai
980-8577, Japan
;

#========================================================================
#  CRYSTAL DATA
#======================================================================== 


#==============================================================================
data_Na3CaBa2P3O12  

_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
Trisodium Monocalcium Dibarium Triphosphorous Dodecaoxygen
; 
_chemical_name_common   
; 
sodium calcium barium phosphate
; 
 
_chemical_formula_structural     'Na2 (Na0.5Ca0.5)2 Ba2 (P O4)3'
_chemical_formula_moiety         'Ba2 Ca Na3 O12 P3' 
_chemical_formula_sum            'Ba2 Ca Na3 O12 P3' 
_chemical_formula_weight          668.64 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'P'  'P'   0.1023   0.0942 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ba'  'Ba'  -0.3244   2.2819 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            trigonal
_symmetry_space_group_name_H-M    'P 3 1 c'
_symmetry_space_group_name_hall   'P 3 -2c'
_symmetry_Int_Tables_number       159
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-y, x-y, z' 
 'y, x, z+1/2' 
 '-x+y, -x, z' 
 '-x, -x+y, z+1/2' 
 'x-y, -y, z+1/2' 
 
_cell_length_a                    5.4515(2) 
_cell_length_b                    5.4515(2) 
_cell_length_c                    23.1283(8) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 120.00 
_cell_volume                      595.26(4) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     3902 
_cell_measurement_theta_min        3.525 
_cell_measurement_theta_max       27.45 
 
_exptl_crystal_description        platelet 
_exptl_crystal_colour             colorless 
_exptl_crystal_size_max           0.106 
_exptl_crystal_size_mid           0.101 
_exptl_crystal_size_min           0.037 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.730 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              612 
_exptl_absorpt_coefficient_mu     7.579 
_exptl_absorpt_correction_type    numerical
_exptl_absorpt_correction_T_min   0.582105 
_exptl_absorpt_correction_T_max   0.796507 
_exptl_absorpt_process_details
;
(NUMABS; Higashi, 1999)
;
 
loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
-0.20  -0.22  23.07     0.0152
-0.47   0.92 -22.80     0.0137
 0.20   0.22 -23.07     0.0152
 1.88  -5.36  -1.18     0.0446
-3.62  -1.70  -1.75     0.0378
-5.35   3.56  -0.55     0.0241
-1.83   5.35   1.20     0.0287
 1.63   3.67   1.76     0.0418
 5.43  -2.50   0.94     0.0445
 4.62  -4.81  -0.10     0.0353


#========================================================================
#  EXPERIMENTAL DATA
#========================================================================

_exptl_special_details 
; 
 ? 
; 

_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71075 
_diffrn_radiation_type            MoK\a
_diffrn_radiation_source          'fine-focus sealed tube'
_diffrn_radiation_monochromator   graphite
_diffrn_measurement_device_type   'Rigaku RAXIS-RAPID II'
_diffrn_measurement_method        ω
_diffrn_detector_area_resol_mean  10.0
_diffrn_reflns_number             5929 
_diffrn_reflns_av_R_equivalents   0.0303 
_diffrn_reflns_av_sigmaI/netI     0.0215 
_diffrn_reflns_limit_h_min        -7 
_diffrn_reflns_limit_h_max        7 
_diffrn_reflns_limit_k_min        -6 
_diffrn_reflns_limit_k_max        7 
_diffrn_reflns_limit_l_min        -30 
_diffrn_reflns_limit_l_max        30 
_diffrn_reflns_theta_min          3.52 
_diffrn_reflns_theta_max          27.45 
_diffrn_measured_fraction_theta_max    0.998 
_diffrn_reflns_theta_full              27.45 
_diffrn_measured_fraction_theta_full   0.998 

_reflns_number_total              924 
_reflns_number_gt                 756 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_cell_refinement        'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_data_reduction         'RAPID-AUTO (Rigaku/MSC, 2005)'
_computing_structure_solution     'SIR2004 (Burla et al., 2005)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics     'VESTA (Momma & Izumi, 2008)'
_computing_publication_material   'SHELXL-97 (Sheldrick, 2008)'

#========================================================================
# Refinement Data
#========================================================================
_iucr_refine_instruction_details
;
TITL     Na3CaBa2P3O12  (NaBa0.666Ca0.333PO4)  P31c1  no159
CELL  0.71075  5.4515  5.4515 23.1283   90.000  90.0  120.000
ZERR     2.00  0.0002  0.0002  0.0008    0.000   0.0    0.000
LATT   -1
SYMM   -Y,+X-Y,+Z
SYMM   +Y,+X,1/2+Z
SYMM   -X+Y,-X,+Z
SYMM   -X,-X+Y,1/2+Z
SYMM   +X-Y,-Y,1/2+Z
SFAC        O       NA      P       CA      BA
UNIT        24       6       6       2       4
L.S.      8
acta
rem   3   3   2         -0.99        349.65       4.71       0.061       0.91
rem   3   4   2         -1.58        147.01       3.93       0.040       0.77
omit  3   3   2
omit  3   4   2
EADP NA1 NA12
EADP O4 O5
EXYZ NA2 CA2
EADP NA2 CA2
EXYZ NA4 CA4
EADP NA4 CA4
SUMP  1.00  0.001  2.0 2
twin  1 0 0 0 1 0 0 0 -1
WGHT      0.0254      4.0376 
BASF   0.50054
FVAR       0.33377
NA1   2    0.333333    0.666667    0.122182    10.16667    0.00946    0.00946 =
         0.01737    0.00000    0.00000    0.00473
NA12  2    0.333333    0.666667    0.088195    10.16667    0.00946    0.00946 =
         0.01737    0.00000    0.00000    0.00473
NA2   2    0.333333    0.666667    0.404177    10.16667    0.02502    0.02502 =
         0.00832    0.00000    0.00000    0.01251
CA2   4    0.333333    0.666667    0.404177    10.16667    0.02502    0.02502 =
         0.00832    0.00000    0.00000    0.01251
NA3   2    0.333333    0.666667    0.710176    10.33333    0.03415    0.03415 =
         0.02006    0.00000    0.00000    0.01708
NA4   2    0.000000    0.000000    0.159063    10.16667    0.00995    0.00995 =
         0.01136    0.00000    0.00000    0.00498
CA4   4    0.000000    0.000000    0.159063    10.16667    0.00995    0.00995 =
         0.01136    0.00000    0.00000    0.00498
BA1   5    0.000000    0.000000   -0.000025    10.33333    0.02649    0.02649 =
         0.01366    0.00000    0.00000    0.01325
BA2   5    0.000000    0.000000    0.317929    10.33333    0.02642    0.02642 =
         0.00720    0.00000    0.00000    0.01321
P1    3    0.333333    0.666667    0.244070    10.33333    0.02893    0.02893 =
         0.00435    0.00000    0.00000    0.01447
P2    3    0.333333    0.666667    0.571936    10.33333    0.00704    0.00704 =
         0.01757    0.00000    0.00000    0.00352
P3    3    0.333333    0.666667    0.888713    10.33333    0.01462    0.01462 =
         0.01816    0.00000    0.00000    0.00731
O1    1    0.370519    0.110390    0.096755    11.00000    0.01769
O2    1    0.255399    0.376687    0.222683    11.00000    0.03677
O3    1    0.362911    0.141122    0.408798    11.00000    0.02252
O4    1    0.333333    0.666667    0.309474    10.33333    0.07120    0.07120 =
         0.02234    0.00000    0.00000    0.03560
O5    1    0.333333    0.666667    0.505952    10.33333    0.07120    0.07120 =
         0.02234    0.00000    0.00000    0.03560
O6    1    0.333333    0.666667    0.821790    10.33333    0.02352    0.02352 =
         0.01454    0.00000    0.00000    0.01176
HKLF      4
END  
;

_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0254P)²+4.0376P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_abs_structure_details 
 'Flack H D (1983), Acta Cryst. A39, 876-881' 
_refine_ls_abs_structure_Flack    0.43(18) 
_refine_ls_number_reflns          924 
_refine_ls_number_parameters      49 
_refine_ls_number_restraints      2 
_refine_ls_R_factor_all           0.0388 
_refine_ls_R_factor_gt            0.0286 
_refine_ls_wR_factor_ref          0.0744 
_refine_ls_wR_factor_gt           0.0659 
_refine_ls_goodness_of_fit_ref    1.204 
_refine_ls_restrained_S_all       1.203 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
_refine_diff_density_max    1.172 
_refine_diff_density_min   -0.858 
_refine_diff_density_rms    0.166 

 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Na1 Na 0.3333 0.6667 0.1222(6) 0.012(2) Uani 0.50 3 d SP . . 
Na12 Na 0.3333 0.6667 0.0882(7) 0.012(2) Uani 0.50 3 d SP . . 
Na2 Na 0.3333 0.6667 0.4042(4) 0.0195(10) Uani 0.50 3 d SP . . 
Ca2 Ca 0.3333 0.6667 0.4042(4) 0.0195(10) Uani 0.50 3 d SP . . 
Na3 Na 0.3333 0.6667 0.7102(3) 0.029(3) Uani 1 3 d S . . 
Na4 Na 0.0000 0.0000 0.1591(7) 0.0104(5) Uani 0.50 3 d SP . . 
Ca4 Ca 0.0000 0.0000 0.1591(7) 0.0104(5) Uani 0.50 3 d SP . . 
Ba1 Ba 0.0000 0.0000 -0.00003(4) 0.0222(6) Uani 1 3 d S . . 
Ba2 Ba 0.0000 0.0000 0.31793(2) 0.0200(5) Uani 1 3 d S . . 
P1 P 0.3333 0.6667 0.2441(4) 0.0208(15) Uani 1 3 d S . . 
P2 P 0.3333 0.6667 0.5719(4) 0.0105(12) Uani 1 3 d S . . 
P3 P 0.3333 0.6667 0.88873(19) 0.0158(9) Uani 1 3 d S . . 
O1 O 0.370(2) 0.110(2) 0.0968(4) 0.018(2) Uiso 1 1 d . . . 
O2 O 0.255(3) 0.377(3) 0.2227(5) 0.037(3) Uiso 1 1 d . . . 
O3 O 0.3629(11) 0.1412(15) 0.4088(6) 0.0225(14) Uiso 1 1 d . . . 
O4 O 0.3333 0.6667 0.3096(9) 0.055(3) Uani 1 3 d S . . 
O5 O 0.3333 0.6667 0.5060(10) 0.055(3) Uani 1 3 d S . . 
O6 O 0.3333 0.6667 0.8218(6) 0.020(2) Uani 1 3 d S . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Na1 Na12 0.79(2) . ? 
Na1 O1 2.398(10) 2 ? 
Na1 O1 2.398(10) 1_565 ? 
Na1 O1 2.398(10) 4_665 ? 
Na1 O2 2.722(16) 4_565 ? 
Na1 O2 2.722(16) 2_665 ? 
Na1 O2 2.722(16) . ? 
Na1 P1 2.819(14) . ? 
Na1 Ca4 3.261(5) 1_565 ? 
Na1 Na4 3.261(5) 1_565 ? 
Na1 Na4 3.261(5) . ? 
Na12 O1 2.333(10) 1_565 ? 
Na12 O1 2.333(10) 2 ? 
Na12 O1 2.333(10) 4_665 ? 
Na12 P2 3.170(2) 3_554 ? 
Na12 P2 3.170(2) 3_454 ? 
Na12 P2 3.170(2) 3_564 ? 
Na12 Na4 3.549(12) . ? 
Na12 Ca4 3.549(12) 1_565 ? 
Na12 Na4 3.549(12) 1_565 ? 
Na12 Ca4 3.549(12) 1_665 ? 
Na2 O4 2.19(2) . ? 
Na2 O5 2.36(2) . ? 
Na2 O3 2.512(7) 1_565 ? 
Na2 O3 2.512(8) 2 ? 
Na2 O3 2.512(7) 4_665 ? 
Na2 O3 2.951(8) 4_565 ? 
Na2 O3 2.951(8) 2_665 ? 
Na2 O3 2.951(8) . ? 
Na2 P3 3.1676(11) 3_554 ? 
Na2 P3 3.1677(11) 3_454 ? 
Na2 P3 3.1677(11) 3_564 ? 
Na2 Ba2 3.726(4) 1_565 ? 
Na3 O2 2.387(13) 3 ? 
Na3 O2 2.387(13) 5_665 ? 
Na3 O2 2.387(13) 6_565 ? 
Na3 O6 2.581(14) . ? 
Na3 O1 3.001(13) 3 ? 
Na3 O1 3.001(12) 6_565 ? 
Na3 O1 3.001(12) 5_665 ? 
Na3 P2 3.198(10) . ? 
Na3 P1 3.243(2) 3 ? 
Na3 P1 3.243(2) 3_565 ? 
Na3 P1 3.243(2) 3_455 ? 
Na3 Na4 3.362(6) 3_565 ? 
Na4 O1 2.303(14) . ? 
Na4 O1 2.303(14) 4 ? 
Na4 O1 2.303(14) 2 ? 
Na4 O2 2.337(16) 2 ? 
Na4 O2 2.337(16) 4 ? 
Na4 O2 2.337(16) . ? 
Na4 Na1 3.261(5) 1_445 ? 
Na4 Na1 3.261(5) 1_545 ? 
Na4 Na3 3.362(6) 3_554 ? 
Na4 Na3 3.362(6) 3_444 ? 
Na4 Na3 3.362(6) 3_454 ? 
Ba1 O3 2.726(10) 6_554 ? 
Ba1 O3 2.726(10) 5_554 ? 
Ba1 O3 2.726(10) 3_554 ? 
Ba1 O1 2.870(10) 2 ? 
Ba1 O1 2.870(10) 4 ? 
Ba1 O1 2.870(10) . ? 
Ba1 O5 3.1505(11) 3_554 ? 
Ba1 O5 3.1505(11) 3_444 ? 
Ba1 O5 3.1506(11) 3_454 ? 
Ba1 P2 3.560(4) 3_554 ? 
Ba1 P2 3.560(4) 3_444 ? 
Ba1 P2 3.560(4) 3_454 ? 
Ba2 O3 2.720(11) 2 ? 
Ba2 O3 2.720(11) 4 ? 
Ba2 O3 2.720(11) . ? 
Ba2 O2 2.855(12) . ? 
Ba2 O2 2.855(12) 2 ? 
Ba2 O2 2.855(12) 4 ? 
Ba2 O6 3.1487(4) 3_554 ? 
Ba2 O6 3.1487(4) 3_444 ? 
Ba2 O6 3.1487(4) 3_454 ? 
Ba2 O4 3.1534(13) 1_445 ? 
Ba2 O4 3.1534(14) . ? 
Ba2 O4 3.1534(13) 1_545 ? 
P1 O2 1.500(14) . ? 
P1 O2 1.500(14) 4_565 ? 
P1 O2 1.501(14) 2_665 ? 
P1 O4 1.514(19) . ? 
P1 Na3 3.243(2) 3_554 ? 
P1 Na3 3.243(2) 3_454 ? 
P1 Na3 3.243(2) 3_564 ? 
P1 Ba2 3.581(4) 1_565 ? 
P1 Ba2 3.581(4) 1_665 ? 
P2 O5 1.52(2) . ? 
P2 O1 1.566(11) 6_565 ? 
P2 O1 1.566(11) 3 ? 
P2 O1 1.566(11) 5_665 ? 
P2 Na12 3.170(2) 3 ? 
P2 Na12 3.170(2) 3_565 ? 
P2 Na12 3.170(2) 3_455 ? 
P2 Na1 3.355(5) 3 ? 
P2 Na1 3.355(5) 3_565 ? 
P2 Na1 3.355(5) 3_455 ? 
P2 Ba1 3.560(4) 3_565 ? 
P3 O3 1.523(6) 5_665 ? 
P3 O3 1.523(7) 3 ? 
P3 O3 1.523(6) 6_565 ? 
P3 O6 1.548(12) . ? 
P3 Na2 3.1676(11) 3 ? 
P3 Ca2 3.1676(11) 3 ? 
P3 Na2 3.1677(11) 3_565 ? 
P3 Ca2 3.1677(11) 3_565 ? 
P3 Ca2 3.1676(11) 3_455 ? 
P3 Na2 3.1676(11) 3_455 ? 
P3 Ba2 3.548(2) 3_565 ? 
P3 Ba2 3.548(2) 3 ? 
O1 P2 1.566(11) 3_554 ? 
O1 Na12 2.333(10) 1_545 ? 
O1 Na1 2.398(10) 1_545 ? 
O1 Na3 3.001(12) 3_554 ? 
O2 Na3 2.387(13) 3_554 ? 
O3 P3 1.523(6) 3_554 ? 
O3 Ca2 2.512(7) 1_545 ? 
O3 Na2 2.512(7) 1_545 ? 
O3 Ba1 2.726(10) 3 ? 
O4 Ba2 3.1534(13) 1_565 ? 
O4 Ba2 3.1534(13) 1_665 ? 
O5 Ba1 3.1505(11) 3_565 ? 
O5 Ba1 3.1505(11) 3 ? 
O5 Ba1 3.1505(11) 3_665 ? 
O6 Ba2 3.1487(4) 3_565 ? 
O6 Ba2 3.1487(4) 3_665 ? 
O6 Ba2 3.1487(4) 3 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
Na12 Na1 O1 75.8(4) . 2 ? 
Na12 Na1 O1 75.8(4) . 1_565 ? 
O1 Na1 O1 114.2(3) 2 1_565 ? 
Na12 Na1 O1 75.8(4) . 4_665 ? 
O1 Na1 O1 114.2(3) 2 4_665 ? 
O1 Na1 O1 114.2(3) 1_565 4_665 ? 
Na12 Na1 O2 148.6(3) . 4_565 ? 
O1 Na1 O2 92.5(4) 2 4_565 ? 
O1 Na1 O2 83.1(3) 1_565 4_565 ? 
O1 Na1 O2 134.8(6) 4_665 4_565 ? 
Na12 Na1 O2 148.6(3) . 2_665 ? 
O1 Na1 O2 134.8(6) 2 2_665 ? 
O1 Na1 O2 92.5(4) 1_565 2_665 ? 
O1 Na1 O2 83.1(3) 4_665 2_665 ? 
O2 Na1 O2 53.6(5) 4_565 2_665 ? 
Na12 Na1 O2 148.6(3) . . ? 
O1 Na1 O2 83.1(3) 2 . ? 
O1 Na1 O2 134.8(6) 1_565 . ? 
O1 Na1 O2 92.5(4) 4_665 . ? 
O2 Na1 O2 53.6(5) 4_565 . ? 
O2 Na1 O2 53.6(5) 2_665 . ? 
Na12 Na1 P1 180.000(2) . . ? 
O1 Na1 P1 104.2(4) 2 . ? 
O1 Na1 P1 104.2(4) 1_565 . ? 
O1 Na1 P1 104.2(4) 4_665 . ? 
O2 Na1 P1 31.4(3) 4_565 . ? 
O2 Na1 P1 31.4(3) 2_665 . ? 
O2 Na1 P1 31.4(3) . . ? 
Na12 Na1 Ca4 105.2(3) . 1_565 ? 
O1 Na1 Ca4 89.6(3) 2 1_565 ? 
O1 Na1 Ca4 44.9(3) 1_565 1_565 ? 
O1 Na1 Ca4 155.2(3) 4_665 1_565 ? 
O2 Na1 Ca4 44.9(4) 4_565 1_565 ? 
O2 Na1 Ca4 84.7(4) 2_665 1_565 ? 
O2 Na1 Ca4 97.6(5) . 1_565 ? 
P1 Na1 Ca4 74.8(3) . 1_565 ? 
Na12 Na1 Na4 105.2(3) . 1_565 ? 
O1 Na1 Na4 89.6(3) 2 1_565 ? 
O1 Na1 Na4 44.9(3) 1_565 1_565 ? 
O1 Na1 Na4 155.2(3) 4_665 1_565 ? 
O2 Na1 Na4 44.9(4) 4_565 1_565 ? 
O2 Na1 Na4 84.7(4) 2_665 1_565 ? 
O2 Na1 Na4 97.6(5) . 1_565 ? 
P1 Na1 Na4 74.8(3) . 1_565 ? 
Ca4 Na1 Na4 0.0(5) 1_565 1_565 ? 
Na12 Na1 Na4 105.2(3) . . ? 
O1 Na1 Na4 44.9(3) 2 . ? 
O1 Na1 Na4 155.2(3) 1_565 . ? 
O1 Na1 Na4 89.6(3) 4_665 . ? 
O2 Na1 Na4 84.7(4) 4_565 . ? 
O2 Na1 Na4 97.6(5) 2_665 . ? 
O2 Na1 Na4 44.9(4) . . ? 
P1 Na1 Na4 74.8(3) . . ? 
Ca4 Na1 Na4 113.4(3) 1_565 . ? 
Na4 Na1 Na4 113.4(3) 1_565 . ? 
Na1 Na12 O1 85.1(4) . 1_565 ? 
Na1 Na12 O1 85.1(4) . 2 ? 
O1 Na12 O1 119.28(12) 1_565 2 ? 
Na1 Na12 O1 85.1(4) . 4_665 ? 
O1 Na12 O1 119.28(12) 1_565 4_665 ? 
O1 Na12 O1 119.28(12) 2 4_665 ? 
Na1 Na12 P2 96.8(3) . 3_554 ? 
O1 Na12 P2 145.8(3) 1_565 3_554 ? 
O1 Na12 P2 94.9(3) 2 3_554 ? 
O1 Na12 P2 28.2(3) 4_665 3_554 ? 
Na1 Na12 P2 96.8(3) . 3_454 ? 
O1 Na12 P2 94.9(3) 1_565 3_454 ? 
O1 Na12 P2 28.2(3) 2 3_454 ? 
O1 Na12 P2 145.8(3) 4_665 3_454 ? 
P2 Na12 P2 118.62(14) 3_554 3_454 ? 
Na1 Na12 P2 96.8(3) . 3_564 ? 
O1 Na12 P2 28.2(3) 1_565 3_564 ? 
O1 Na12 P2 145.8(3) 2 3_564 ? 
O1 Na12 P2 94.9(3) 4_665 3_564 ? 
P2 Na12 P2 118.62(14) 3_554 3_564 ? 
P2 Na12 P2 118.62(14) 3_454 3_564 ? 
Na1 Na12 Na4 62.5(4) . . ? 
O1 Na12 Na4 139.2(6) 1_565 . ? 
O1 Na12 Na4 39.7(3) 2 . ? 
O1 Na12 Na4 83.9(3) 4_665 . ? 
P2 Na12 Na4 67.32(11) 3_554 . ? 
P2 Na12 Na4 67.32(11) 3_454 . ? 
P2 Na12 Na4 159.3(7) 3_564 . ? 
Na1 Na12 Ca4 62.5(4) . 1_565 ? 
O1 Na12 Ca4 39.7(3) 1_565 1_565 ? 
O1 Na12 Ca4 83.9(3) 2 1_565 ? 
O1 Na12 Ca4 139.2(6) 4_665 1_565 ? 
P2 Na12 Ca4 159.3(7) 3_554 1_565 ? 
P2 Na12 Ca4 67.32(11) 3_454 1_565 ? 
P2 Na12 Ca4 67.32(11) 3_564 1_565 ? 
Na4 Na12 Ca4 100.4(5) . 1_565 ? 
Na1 Na12 Na4 62.5(4) . 1_565 ? 
O1 Na12 Na4 39.7(3) 1_565 1_565 ? 
O1 Na12 Na4 83.9(3) 2 1_565 ? 
O1 Na12 Na4 139.2(6) 4_665 1_565 ? 
P2 Na12 Na4 159.3(7) 3_554 1_565 ? 
P2 Na12 Na4 67.32(11) 3_454 1_565 ? 
P2 Na12 Na4 67.32(11) 3_564 1_565 ? 
Na4 Na12 Na4 100.4(5) . 1_565 ? 
Ca4 Na12 Na4 0.0(5) 1_565 1_565 ? 
Na1 Na12 Ca4 62.5(4) . 1_665 ? 
O1 Na12 Ca4 83.9(3) 1_565 1_665 ? 
O1 Na12 Ca4 139.2(6) 2 1_665 ? 
O1 Na12 Ca4 39.7(3) 4_665 1_665 ? 
P2 Na12 Ca4 67.32(11) 3_554 1_665 ? 
P2 Na12 Ca4 159.3(7) 3_454 1_665 ? 
P2 Na12 Ca4 67.32(11) 3_564 1_665 ? 
Na4 Na12 Ca4 100.4(5) . 1_665 ? 
Ca4 Na12 Ca4 100.4(5) 1_565 1_665 ? 
Na4 Na12 Ca4 100.4(5) 1_565 1_665 ? 
O4 Na2 O5 180.000(5) . . ? 
O4 Na2 O3 92.4(3) . 1_565 ? 
O5 Na2 O3 87.6(3) . 1_565 ? 
O4 Na2 O3 92.4(3) . 2 ? 
O5 Na2 O3 87.6(3) . 2 ? 
O3 Na2 O3 119.82(5) 1_565 2 ? 
O4 Na2 O3 92.4(3) . 4_665 ? 
O5 Na2 O3 87.6(3) . 4_665 ? 
O3 Na2 O3 119.82(5) 1_565 4_665 ? 
O3 Na2 O3 119.82(5) 2 4_665 ? 
O4 Na2 O3 92.1(3) . 4_565 ? 
O5 Na2 O3 87.9(3) . 4_565 ? 
O3 Na2 O3 65.9(2) 1_565 4_565 ? 
O3 Na2 O3 54.0(2) 2 4_565 ? 
O3 Na2 O3 172.6(4) 4_665 4_565 ? 
O4 Na2 O3 92.1(3) . 2_665 ? 
O5 Na2 O3 87.9(3) . 2_665 ? 
O3 Na2 O3 54.0(2) 1_565 2_665 ? 
O3 Na2 O3 172.6(4) 2 2_665 ? 
O3 Na2 O3 65.9(2) 4_665 2_665 ? 
O3 Na2 O3 119.87(4) 4_565 2_665 ? 
O4 Na2 O3 92.1(3) . . ? 
O5 Na2 O3 87.9(3) . . ? 
O3 Na2 O3 172.6(4) 1_565 . ? 
O3 Na2 O3 65.9(2) 2 . ? 
O3 Na2 O3 54.0(2) 4_665 . ? 
O3 Na2 O3 119.87(4) 4_565 . ? 
O3 Na2 O3 119.87(4) 2_665 . ? 
O4 Na2 P3 83.52(17) . 3_554 ? 
O5 Na2 P3 96.48(17) . 3_554 ? 
O3 Na2 P3 146.67(13) 1_565 3_554 ? 
O3 Na2 P3 93.44(13) 2 3_554 ? 
O3 Na2 P3 28.21(14) 4_665 3_554 ? 
O3 Na2 P3 147.09(11) 4_565 3_554 ? 
O3 Na2 P3 92.93(11) 2_665 3_554 ? 
O3 Na2 P3 28.55(12) . 3_554 ? 
O4 Na2 P3 83.52(17) . 3_454 ? 
O5 Na2 P3 96.48(17) . 3_454 ? 
O3 Na2 P3 93.44(13) 1_565 3_454 ? 
O3 Na2 P3 28.21(14) 2 3_454 ? 
O3 Na2 P3 146.67(13) 4_665 3_454 ? 
O3 Na2 P3 28.55(12) 4_565 3_454 ? 
O3 Na2 P3 147.09(11) 2_665 3_454 ? 
O3 Na2 P3 92.93(11) . 3_454 ? 
P3 Na2 P3 118.74(7) 3_554 3_454 ? 
O4 Na2 P3 83.52(17) . 3_564 ? 
O5 Na2 P3 96.48(17) . 3_564 ? 
O3 Na2 P3 28.21(14) 1_565 3_564 ? 
O3 Na2 P3 146.67(13) 2 3_564 ? 
O3 Na2 P3 93.45(13) 4_665 3_564 ? 
O3 Na2 P3 92.93(11) 4_565 3_564 ? 
O3 Na2 P3 28.55(12) 2_665 3_564 ? 
O3 Na2 P3 147.09(12) . 3_564 ? 
P3 Na2 P3 118.74(7) 3_554 3_564 ? 
P3 Na2 P3 118.74(7) 3_454 3_564 ? 
O4 Na2 Ba2 57.63(11) . 1_565 ? 
O5 Na2 Ba2 122.37(11) . 1_565 ? 
O3 Na2 Ba2 46.9(3) 1_565 1_565 ? 
O3 Na2 Ba2 88.6(2) 2 1_565 ? 
O3 Na2 Ba2 140.9(3) 4_665 1_565 ? 
O3 Na2 Ba2 46.3(2) 4_565 1_565 ? 
O3 Na2 Ba2 88.82(17) 2_665 1_565 ? 
O3 Na2 Ba2 140.3(3) . 1_565 ? 
P3 Na2 Ba2 141.2(3) 3_554 1_565 ? 
P3 Na2 Ba2 61.31(8) 3_454 1_565 ? 
P3 Na2 Ba2 61.31(8) 3_564 1_565 ? 
O2 Na3 O2 118.56(15) 3 5_665 ? 
O2 Na3 O2 118.56(15) 3 6_565 ? 
O2 Na3 O2 118.56(14) 5_665 6_565 ? 
O2 Na3 O6 83.1(3) 3 . ? 
O2 Na3 O6 83.1(3) 5_665 . ? 
O2 Na3 O6 83.1(3) 6_565 . ? 
O2 Na3 O1 78.7(3) 3 3 ? 
O2 Na3 O1 125.6(5) 5_665 3 ? 
O2 Na3 O1 86.1(4) 6_565 3 ? 
O6 Na3 O1 151.0(2) . 3 ? 
O2 Na3 O1 125.6(5) 3 6_565 ? 
O2 Na3 O1 86.1(4) 5_665 6_565 ? 
O2 Na3 O1 78.7(3) 6_565 6_565 ? 
O6 Na3 O1 151.0(2) . 6_565 ? 
O1 Na3 O1 49.7(4) 3 6_565 ? 
O2 Na3 O1 86.1(4) 3 5_665 ? 
O2 Na3 O1 78.7(3) 5_665 5_665 ? 
O2 Na3 O1 125.6(5) 6_565 5_665 ? 
O6 Na3 O1 151.0(2) . 5_665 ? 
O1 Na3 O1 49.7(4) 3 5_665 ? 
O1 Na3 O1 49.7(4) 6_565 5_665 ? 
O2 Na3 P2 96.9(3) 3 . ? 
O2 Na3 P2 96.9(3) 5_665 . ? 
O2 Na3 P2 96.9(3) 6_565 . ? 
O6 Na3 P2 180.000(3) . . ? 
O1 Na3 P2 29.0(2) 3 . ? 
O1 Na3 P2 29.0(2) 6_565 . ? 
O1 Na3 P2 29.0(2) 5_665 . ? 
O2 Na3 P1 25.6(3) 3 3 ? 
O2 Na3 P1 93.1(3) 5_665 3 ? 
O2 Na3 P1 139.5(3) 6_565 3 ? 
O6 Na3 P1 76.02(17) . 3 ? 
O1 Na3 P1 95.7(2) 3 3 ? 
O1 Na3 P1 131.6(3) 6_565 3 ? 
O1 Na3 P1 82.6(2) 5_665 3 ? 
P2 Na3 P1 103.98(17) . 3 ? 
O2 Na3 P1 139.5(4) 3 3_565 ? 
O2 Na3 P1 25.6(3) 5_665 3_565 ? 
O2 Na3 P1 93.1(3) 6_565 3_565 ? 
O6 Na3 P1 76.02(18) . 3_565 ? 
O1 Na3 P1 131.6(3) 3 3_565 ? 
O1 Na3 P1 82.6(2) 6_565 3_565 ? 
O1 Na3 P1 95.7(2) 5_665 3_565 ? 
P2 Na3 P1 103.98(17) . 3_565 ? 
P1 Na3 P1 114.36(14) 3 3_565 ? 
O2 Na3 P1 93.1(3) 3 3_455 ? 
O2 Na3 P1 139.5(3) 5_665 3_455 ? 
O2 Na3 P1 25.6(3) 6_565 3_455 ? 
O6 Na3 P1 76.02(17) . 3_455 ? 
O1 Na3 P1 82.6(2) 3 3_455 ? 
O1 Na3 P1 95.7(2) 6_565 3_455 ? 
O1 Na3 P1 131.6(3) 5_665 3_455 ? 
P2 Na3 P1 103.98(18) . 3_455 ? 
P1 Na3 P1 114.36(14) 3 3_455 ? 
P1 Na3 P1 114.36(13) 3_565 3_455 ? 
O2 Na3 Na4 152.2(4) 3 3_565 ? 
O2 Na3 Na4 87.8(3) 5_665 3_565 ? 
O2 Na3 Na4 44.0(3) 6_565 3_565 ? 
O6 Na3 Na4 110.6(3) . 3_565 ? 
O1 Na3 Na4 78.5(3) 3 3_565 ? 
O1 Na3 Na4 41.9(3) 6_565 3_565 ? 
O1 Na3 Na4 91.2(3) 5_665 3_565 ? 
P2 Na3 Na4 69.4(3) . 3_565 ? 
P1 Na3 Na4 173.4(4) 3 3_565 ? 
P1 Na3 Na4 68.33(10) 3_565 3_565 ? 
P1 Na3 Na4 68.33(10) 3_455 3_565 ? 
O1 Na4 O1 85.0(6) . 4 ? 
O1 Na4 O1 85.0(6) . 2 ? 
O1 Na4 O1 85.0(6) 4 2 ? 
O1 Na4 O2 178.8(6) . 2 ? 
O1 Na4 O2 94.4(4) 4 2 ? 
O1 Na4 O2 96.0(4) 2 2 ? 
O1 Na4 O2 94.4(4) . 4 ? 
O1 Na4 O2 96.0(4) 4 4 ? 
O1 Na4 O2 178.8(6) 2 4 ? 
O2 Na4 O2 84.6(6) 2 4 ? 
O1 Na4 O2 96.0(4) . . ? 
O1 Na4 O2 178.8(6) 4 . ? 
O1 Na4 O2 94.4(4) 2 . ? 
O2 Na4 O2 84.6(6) 2 . ? 
O2 Na4 O2 84.6(6) 4 . ? 
O1 Na4 Na1 124.7(7) . 1_445 ? 
O1 Na4 Na1 47.3(3) 4 1_445 ? 
O1 Na4 Na1 67.5(3) 2 1_445 ? 
O2 Na4 Na1 55.3(4) 2 1_445 ? 
O2 Na4 Na1 113.7(4) 4 1_445 ? 
O2 Na4 Na1 131.5(5) . 1_445 ? 
O1 Na4 Na1 67.5(3) . . ? 
O1 Na4 Na1 124.7(7) 4 . ? 
O1 Na4 Na1 47.3(3) 2 . ? 
O2 Na4 Na1 113.7(4) 2 . ? 
O2 Na4 Na1 131.5(5) 4 . ? 
O2 Na4 Na1 55.3(4) . . ? 
Na1 Na4 Na1 113.4(3) 1_445 . ? 
O1 Na4 Na1 47.3(3) . 1_545 ? 
O1 Na4 Na1 67.5(3) 4 1_545 ? 
O1 Na4 Na1 124.7(7) 2 1_545 ? 
O2 Na4 Na1 131.5(5) 2 1_545 ? 
O2 Na4 Na1 55.3(4) 4 1_545 ? 
O2 Na4 Na1 113.7(4) . 1_545 ? 
Na1 Na4 Na1 113.4(3) 1_445 1_545 ? 
Na1 Na4 Na1 113.4(3) . 1_545 ? 
O1 Na4 Na3 60.6(3) . 3_554 ? 
O1 Na4 Na3 136.0(3) 4 3_554 ? 
O1 Na4 Na3 115.6(3) 2 3_554 ? 
O2 Na4 Na3 119.4(6) 2 3_554 ? 
O2 Na4 Na3 63.2(4) 4 3_554 ? 
O2 Na4 Na3 45.2(3) . 3_554 ? 
Na1 Na4 Na3 174.6(6) 1_445 3_554 ? 
Na1 Na4 Na3 68.92(11) . 3_554 ? 
Na1 Na4 Na3 68.92(11) 1_545 3_554 ? 
O1 Na4 Na3 115.6(3) . 3_444 ? 
O1 Na4 Na3 60.6(3) 4 3_444 ? 
O1 Na4 Na3 136.0(3) 2 3_444 ? 
O2 Na4 Na3 63.2(4) 2 3_444 ? 
O2 Na4 Na3 45.2(3) 4 3_444 ? 
O2 Na4 Na3 119.4(6) . 3_444 ? 
Na1 Na4 Na3 68.92(11) 1_445 3_444 ? 
Na1 Na4 Na3 174.6(6) . 3_444 ? 
Na1 Na4 Na3 68.92(11) 1_545 3_444 ? 
Na3 Na4 Na3 108.3(3) 3_554 3_444 ? 
O1 Na4 Na3 136.0(3) . 3_454 ? 
O1 Na4 Na3 115.6(3) 4 3_454 ? 
O1 Na4 Na3 60.6(3) 2 3_454 ? 
O2 Na4 Na3 45.2(3) 2 3_454 ? 
O2 Na4 Na3 119.4(6) 4 3_454 ? 
O2 Na4 Na3 63.2(4) . 3_454 ? 
Na1 Na4 Na3 68.92(11) 1_445 3_454 ? 
Na1 Na4 Na3 68.92(11) . 3_454 ? 
Na1 Na4 Na3 174.6(6) 1_545 3_454 ? 
Na3 Na4 Na3 108.3(3) 3_554 3_454 ? 
Na3 Na4 Na3 108.3(3) 3_444 3_454 ? 
O3 Ba1 O3 66.6(3) 6_554 5_554 ? 
O3 Ba1 O3 66.6(3) 6_554 3_554 ? 
O3 Ba1 O3 66.6(3) 5_554 3_554 ? 
O3 Ba1 O1 167.2(3) 6_554 2 ? 
O3 Ba1 O1 122.5(3) 5_554 2 ? 
O3 Ba1 O1 107.3(3) 3_554 2 ? 
O3 Ba1 O1 122.5(3) 6_554 4 ? 
O3 Ba1 O1 107.3(3) 5_554 4 ? 
O3 Ba1 O1 167.2(3) 3_554 4 ? 
O1 Ba1 O1 65.6(3) 2 4 ? 
O3 Ba1 O1 107.3(3) 6_554 . ? 
O3 Ba1 O1 167.2(3) 5_554 . ? 
O3 Ba1 O1 122.5(3) 3_554 . ? 
O1 Ba1 O1 65.6(3) 2 . ? 
O1 Ba1 O1 65.6(3) 4 . ? 
O3 Ba1 O5 69.6(4) 6_554 3_554 ? 
O3 Ba1 O5 131.5(5) 5_554 3_554 ? 
O3 Ba1 O5 77.9(4) 3_554 3_554 ? 
O1 Ba1 O5 98.4(4) 2 3_554 ? 
O1 Ba1 O5 113.1(5) 4 3_554 ? 
O1 Ba1 O5 49.9(4) . 3_554 ? 
O3 Ba1 O5 77.9(4) 6_554 3_444 ? 
O3 Ba1 O5 69.6(4) 5_554 3_444 ? 
O3 Ba1 O5 131.5(5) 3_554 3_444 ? 
O1 Ba1 O5 113.1(5) 2 3_444 ? 
O1 Ba1 O5 49.9(4) 4 3_444 ? 
O1 Ba1 O5 98.4(4) . 3_444 ? 
O5 Ba1 O5 119.81(7) 3_554 3_444 ? 
O3 Ba1 O5 131.5(5) 6_554 3_454 ? 
O3 Ba1 O5 77.9(4) 5_554 3_454 ? 
O3 Ba1 O5 69.6(4) 3_554 3_454 ? 
O1 Ba1 O5 49.9(4) 2 3_454 ? 
O1 Ba1 O5 98.4(4) 4 3_454 ? 
O1 Ba1 O5 113.1(5) . 3_454 ? 
O5 Ba1 O5 119.80(7) 3_554 3_454 ? 
O5 Ba1 O5 119.80(7) 3_444 3_454 ? 
O3 Ba1 P2 91.3(2) 6_554 3_554 ? 
O3 Ba1 P2 156.5(3) 5_554 3_554 ? 
O3 Ba1 P2 98.36(19) 3_554 3_554 ? 
O1 Ba1 P2 78.2(2) 2 3_554 ? 
O1 Ba1 P2 90.8(2) 4 3_554 ? 
O1 Ba1 P2 25.4(2) . 3_554 ? 
O5 Ba1 P2 25.3(4) 3_554 3_554 ? 
O5 Ba1 P2 114.9(3) 3_444 3_554 ? 
O5 Ba1 P2 114.9(3) 3_454 3_554 ? 
O3 Ba1 P2 98.37(19) 6_554 3_444 ? 
O3 Ba1 P2 91.3(2) 5_554 3_444 ? 
O3 Ba1 P2 156.5(3) 3_554 3_444 ? 
O1 Ba1 P2 90.8(2) 2 3_444 ? 
O1 Ba1 P2 25.4(2) 4 3_444 ? 
O1 Ba1 P2 78.2(2) . 3_444 ? 
O5 Ba1 P2 114.9(3) 3_554 3_444 ? 
O5 Ba1 P2 25.3(4) 3_444 3_444 ? 
O5 Ba1 P2 114.9(3) 3_454 3_444 ? 
P2 Ba1 P2 99.92(17) 3_554 3_444 ? 
O3 Ba1 P2 156.5(3) 6_554 3_454 ? 
O3 Ba1 P2 98.36(19) 5_554 3_454 ? 
O3 Ba1 P2 91.3(2) 3_554 3_454 ? 
O1 Ba1 P2 25.4(2) 2 3_454 ? 
O1 Ba1 P2 78.2(2) 4 3_454 ? 
O1 Ba1 P2 90.8(2) . 3_454 ? 
O5 Ba1 P2 114.9(3) 3_554 3_454 ? 
O5 Ba1 P2 114.9(3) 3_444 3_454 ? 
O5 Ba1 P2 25.3(4) 3_454 3_454 ? 
P2 Ba1 P2 99.92(17) 3_554 3_454 ? 
P2 Ba1 P2 99.92(17) 3_444 3_454 ? 
O3 Ba2 O3 66.7(3) 2 4 ? 
O3 Ba2 O3 66.7(3) 2 . ? 
O3 Ba2 O3 66.7(3) 4 . ? 
O3 Ba2 O2 114.9(3) 2 . ? 
O3 Ba2 O2 177.3(4) 4 . ? 
O3 Ba2 O2 111.6(3) . . ? 
O3 Ba2 O2 111.6(3) 2 2 ? 
O3 Ba2 O2 114.9(3) 4 2 ? 
O3 Ba2 O2 177.3(4) . 2 ? 
O2 Ba2 O2 66.9(4) . 2 ? 
O3 Ba2 O2 177.3(4) 2 4 ? 
O3 Ba2 O2 111.6(3) 4 4 ? 
O3 Ba2 O2 114.9(3) . 4 ? 
O2 Ba2 O2 66.9(4) . 4 ? 
O2 Ba2 O2 66.9(4) 2 4 ? 
O3 Ba2 O6 102.9(3) 2 3_554 ? 
O3 Ba2 O6 111.3(3) 4 3_554 ? 
O3 Ba2 O6 49.3(3) . 3_554 ? 
O2 Ba2 O6 66.4(3) . 3_554 ? 
O2 Ba2 O6 130.2(3) 2 3_554 ? 
O2 Ba2 O6 79.7(3) 4 3_554 ? 
O3 Ba2 O6 111.3(3) 2 3_444 ? 
O3 Ba2 O6 49.3(3) 4 3_444 ? 
O3 Ba2 O6 102.9(3) . 3_444 ? 
O2 Ba2 O6 130.2(3) . 3_444 ? 
O2 Ba2 O6 79.7(3) 2 3_444 ? 
O2 Ba2 O6 66.4(3) 4 3_444 ? 
O6 Ba2 O6 119.92(2) 3_554 3_444 ? 
O3 Ba2 O6 49.3(3) 2 3_454 ? 
O3 Ba2 O6 102.9(3) 4 3_454 ? 
O3 Ba2 O6 111.3(3) . 3_454 ? 
O2 Ba2 O6 79.7(3) . 3_454 ? 
O2 Ba2 O6 66.4(3) 2 3_454 ? 
O2 Ba2 O6 130.2(3) 4 3_454 ? 
O6 Ba2 O6 119.92(2) 3_554 3_454 ? 
O6 Ba2 O6 119.92(2) 3_444 3_454 ? 
O3 Ba2 O4 78.6(3) 2 1_445 ? 
O3 Ba2 O4 70.3(3) 4 1_445 ? 
O3 Ba2 O4 132.5(5) . 1_445 ? 
O2 Ba2 O4 112.0(4) . 1_445 ? 
O2 Ba2 O4 48.0(4) 2 1_445 ? 
O2 Ba2 O4 98.8(4) 4 1_445 ? 
O6 Ba2 O4 178.1(6) 3_554 1_445 ? 
O6 Ba2 O4 60.19(2) 3_444 1_445 ? 
O6 Ba2 O4 60.19(2) 3_454 1_445 ? 
O3 Ba2 O4 70.3(3) 2 . ? 
O3 Ba2 O4 132.5(5) 4 . ? 
O3 Ba2 O4 78.6(3) . . ? 
O2 Ba2 O4 48.0(4) . . ? 
O2 Ba2 O4 98.8(4) 2 . ? 
O2 Ba2 O4 112.0(4) 4 . ? 
O6 Ba2 O4 60.19(2) 3_554 . ? 
O6 Ba2 O4 178.1(6) 3_444 . ? 
O6 Ba2 O4 60.19(2) 3_454 . ? 
O4 Ba2 O4 119.63(8) 1_445 . ? 
O3 Ba2 O4 132.5(5) 2 1_545 ? 
O3 Ba2 O4 78.6(3) 4 1_545 ? 
O3 Ba2 O4 70.3(3) . 1_545 ? 
O2 Ba2 O4 98.8(4) . 1_545 ? 
O2 Ba2 O4 112.0(4) 2 1_545 ? 
O2 Ba2 O4 48.0(4) 4 1_545 ? 
O6 Ba2 O4 60.19(2) 3_554 1_545 ? 
O6 Ba2 O4 60.19(2) 3_444 1_545 ? 
O6 Ba2 O4 178.1(6) 3_454 1_545 ? 
O4 Ba2 O4 119.63(8) 1_445 1_545 ? 
O4 Ba2 O4 119.63(8) . 1_545 ? 
O2 P1 O2 109.7(5) . 4_565 ? 
O2 P1 O2 109.7(5) . 2_665 ? 
O2 P1 O2 109.7(5) 4_565 2_665 ? 
O2 P1 O4 109.3(5) . . ? 
O2 P1 O4 109.3(5) 4_565 . ? 
O2 P1 O4 109.3(5) 2_665 . ? 
O2 P1 Na1 70.7(5) . . ? 
O2 P1 Na1 70.7(5) 4_565 . ? 
O2 P1 Na1 70.7(5) 2_665 . ? 
O4 P1 Na1 180.000(2) . . ? 
O2 P1 Na3 43.4(5) . 3_554 ? 
O2 P1 Na3 143.7(6) 4_565 3_554 ? 
O2 P1 Na3 71.5(5) 2_665 3_554 ? 
O4 P1 Na3 103.98(17) . 3_554 ? 
Na1 P1 Na3 76.02(17) . 3_554 ? 
O2 P1 Na3 71.5(5) . 3_454 ? 
O2 P1 Na3 43.4(5) 4_565 3_454 ? 
O2 P1 Na3 143.7(6) 2_665 3_454 ? 
O4 P1 Na3 103.98(17) . 3_454 ? 
Na1 P1 Na3 76.02(17) . 3_454 ? 
Na3 P1 Na3 114.36(13) 3_554 3_454 ? 
O2 P1 Na3 143.7(6) . 3_564 ? 
O2 P1 Na3 71.5(5) 4_565 3_564 ? 
O2 P1 Na3 43.4(5) 2_665 3_564 ? 
O4 P1 Na3 103.98(17) . 3_564 ? 
Na1 P1 Na3 76.02(17) . 3_564 ? 
Na3 P1 Na3 114.36(13) 3_554 3_564 ? 
Na3 P1 Na3 114.36(13) 3_454 3_564 ? 
O2 P1 Ba2 49.9(5) . . ? 
O2 P1 Ba2 111.9(5) 4_565 . ? 
O2 P1 Ba2 138.0(5) 2_665 . ? 
O4 P1 Ba2 61.51(13) . . ? 
Na1 P1 Ba2 118.49(13) . . ? 
Na3 P1 Ba2 71.87(8) 3_554 . ? 
Na3 P1 Ba2 71.87(8) 3_454 . ? 
Na3 P1 Ba2 165.5(3) 3_564 . ? 
O2 P1 Ba2 138.0(5) . 1_565 ? 
O2 P1 Ba2 49.9(5) 4_565 1_565 ? 
O2 P1 Ba2 111.9(5) 2_665 1_565 ? 
O4 P1 Ba2 61.51(13) . 1_565 ? 
Na1 P1 Ba2 118.49(13) . 1_565 ? 
Na3 P1 Ba2 165.5(3) 3_554 1_565 ? 
Na3 P1 Ba2 71.87(8) 3_454 1_565 ? 
Na3 P1 Ba2 71.87(8) 3_564 1_565 ? 
Ba2 P1 Ba2 99.13(16) . 1_565 ? 
O2 P1 Ba2 111.9(5) . 1_665 ? 
O2 P1 Ba2 138.0(5) 4_565 1_665 ? 
O2 P1 Ba2 49.9(5) 2_665 1_665 ? 
O4 P1 Ba2 61.51(13) . 1_665 ? 
Na1 P1 Ba2 118.49(13) . 1_665 ? 
Na3 P1 Ba2 71.87(8) 3_554 1_665 ? 
Na3 P1 Ba2 165.5(3) 3_454 1_665 ? 
Na3 P1 Ba2 71.87(8) 3_564 1_665 ? 
Ba2 P1 Ba2 99.13(16) . 1_665 ? 
Ba2 P1 Ba2 99.13(16) 1_565 1_665 ? 
O5 P2 O1 111.5(5) . 6_565 ? 
O5 P2 O1 111.5(5) . 3 ? 
O1 P2 O1 107.4(5) 6_565 3 ? 
O5 P2 O1 111.5(5) . 5_665 ? 
O1 P2 O1 107.4(5) 6_565 5_665 ? 
O1 P2 O1 107.4(5) 3 5_665 ? 
O5 P2 Na12 96.8(3) . 3 ? 
O1 P2 Na12 147.5(6) 6_565 3 ? 
O1 P2 Na12 74.8(4) 3 3 ? 
O1 P2 Na12 44.7(4) 5_665 3 ? 
O5 P2 Na12 96.8(3) . 3_565 ? 
O1 P2 Na12 44.7(4) 6_565 3_565 ? 
O1 P2 Na12 147.5(6) 3 3_565 ? 
O1 P2 Na12 74.8(4) 5_665 3_565 ? 
Na12 P2 Na12 118.62(14) 3 3_565 ? 
O5 P2 Na12 96.8(3) . 3_455 ? 
O1 P2 Na12 74.8(4) 6_565 3_455 ? 
O1 P2 Na12 44.7(4) 3 3_455 ? 
O1 P2 Na12 147.5(6) 5_665 3_455 ? 
Na12 P2 Na12 118.62(14) 3 3_455 ? 
Na12 P2 Na12 118.62(14) 3_565 3_455 ? 
O5 P2 Na3 180.000(4) . . ? 
O1 P2 Na3 68.5(5) 6_565 . ? 
O1 P2 Na3 68.5(5) 3 . ? 
O1 P2 Na3 68.5(5) 5_665 . ? 
Na12 P2 Na3 83.2(3) 3 . ? 
Na12 P2 Na3 83.2(3) 3_565 . ? 
Na12 P2 Na3 83.2(3) 3_455 . ? 
O5 P2 Na1 110.3(2) . 3 ? 
O1 P2 Na1 135.3(5) 6_565 3 ? 
O1 P2 Na1 70.5(4) 3 3 ? 
O1 P2 Na1 40.7(4) 5_665 3 ? 
Na12 P2 Na1 13.5(4) 3 3 ? 
Na12 P2 Na1 115.13(18) 3_565 3 ? 
Na12 P2 Na1 115.13(18) 3_455 3 ? 
Na3 P2 Na1 69.7(2) . 3 ? 
O5 P2 Na1 110.3(2) . 3_565 ? 
O1 P2 Na1 40.7(4) 6_565 3_565 ? 
O1 P2 Na1 135.3(5) 3 3_565 ? 
O1 P2 Na1 70.5(4) 5_665 3_565 ? 
Na12 P2 Na1 115.13(18) 3 3_565 ? 
Na12 P2 Na1 13.5(4) 3_565 3_565 ? 
Na12 P2 Na1 115.13(18) 3_455 3_565 ? 
Na3 P2 Na1 69.7(2) . 3_565 ? 
Na1 P2 Na1 108.7(2) 3 3_565 ? 
O5 P2 Na1 110.3(2) . 3_455 ? 
O1 P2 Na1 70.5(4) 6_565 3_455 ? 
O1 P2 Na1 40.7(4) 3 3_455 ? 
O1 P2 Na1 135.3(5) 5_665 3_455 ? 
Na12 P2 Na1 115.13(18) 3 3_455 ? 
Na12 P2 Na1 115.13(18) 3_565 3_455 ? 
Na12 P2 Na1 13.5(4) 3_455 3_455 ? 
Na3 P2 Na1 69.7(2) . 3_455 ? 
Na1 P2 Na1 108.7(2) 3 3_455 ? 
Na1 P2 Na1 108.7(2) 3_565 3_455 ? 
O5 P2 Ba1 62.13(13) . 3_565 ? 
O1 P2 Ba1 51.8(4) 6_565 3_565 ? 
O1 P2 Ba1 111.5(4) 3 3_565 ? 
O1 P2 Ba1 140.0(4) 5_665 3_565 ? 
Na12 P2 Ba1 158.9(4) 3 3_565 ? 
Na12 P2 Ba1 67.45(17) 3_565 3_565 ? 
Na12 P2 Ba1 67.45(17) 3_455 3_565 ? 
Na3 P2 Ba1 117.87(13) . 3_565 ? 
Na1 P2 Ba1 172.4(3) 3 3_565 ? 
Na1 P2 Ba1 75.36(12) 3_565 3_565 ? 
Na1 P2 Ba1 75.36(12) 3_455 3_565 ? 
O3 P3 O3 111.1(5) 5_665 3 ? 
O3 P3 O3 111.1(5) 5_665 6_565 ? 
O3 P3 O3 111.1(5) 3 6_565 ? 
O3 P3 O6 107.7(5) 5_665 . ? 
O3 P3 O6 107.7(5) 3 . ? 
O3 P3 O6 107.7(5) 6_565 . ? 
O3 P3 Na2 51.2(3) 5_665 3 ? 
O3 P3 Na2 67.8(3) 3 3 ? 
O3 P3 Na2 154.3(6) 6_565 3 ? 
O6 P3 Na2 96.48(17) . 3 ? 
O3 P3 Ca2 51.2(3) 5_665 3 ? 
O3 P3 Ca2 67.8(3) 3 3 ? 
O3 P3 Ca2 154.3(6) 6_565 3 ? 
O6 P3 Ca2 96.48(17) . 3 ? 
Na2 P3 Ca2 0.0(3) 3 3 ? 
O3 P3 Na2 67.8(3) 5_665 3_565 ? 
O3 P3 Na2 154.3(6) 3 3_565 ? 
O3 P3 Na2 51.2(3) 6_565 3_565 ? 
O6 P3 Na2 96.48(17) . 3_565 ? 
Na2 P3 Na2 118.75(7) 3 3_565 ? 
Ca2 P3 Na2 118.75(7) 3 3_565 ? 
O3 P3 Ca2 67.8(3) 5_665 3_565 ? 
O3 P3 Ca2 154.3(6) 3 3_565 ? 
O3 P3 Ca2 51.2(3) 6_565 3_565 ? 
O6 P3 Ca2 96.48(17) . 3_565 ? 
Na2 P3 Ca2 118.75(7) 3 3_565 ? 
Ca2 P3 Ca2 118.75(7) 3 3_565 ? 
Na2 P3 Ca2 0.0(3) 3_565 3_565 ? 
O3 P3 Ca2 154.3(6) 5_665 3_455 ? 
O3 P3 Ca2 51.2(3) 3 3_455 ? 
O3 P3 Ca2 67.8(3) 6_565 3_455 ? 
O6 P3 Ca2 96.48(17) . 3_455 ? 
Na2 P3 Ca2 118.75(7) 3 3_455 ? 
Ca2 P3 Ca2 118.75(7) 3 3_455 ? 
Na2 P3 Ca2 118.74(7) 3_565 3_455 ? 
Ca2 P3 Ca2 118.74(7) 3_565 3_455 ? 
O3 P3 Na2 154.3(6) 5_665 3_455 ? 
O3 P3 Na2 51.2(3) 3 3_455 ? 
O3 P3 Na2 67.8(3) 6_565 3_455 ? 
O6 P3 Na2 96.48(17) . 3_455 ? 
Na2 P3 Na2 118.75(7) 3 3_455 ? 
Ca2 P3 Na2 118.75(7) 3 3_455 ? 
Na2 P3 Na2 118.74(7) 3_565 3_455 ? 
Ca2 P3 Na2 118.74(7) 3_565 3_455 ? 
Ca2 P3 Na2 0.0 3_455 3_455 ? 
O3 P3 Ba2 132.0(3) 5_665 3_565 ? 
O3 P3 Ba2 116.6(3) 3 3_565 ? 
O3 P3 Ba2 46.0(5) 6_565 3_565 ? 
O6 P3 Ba2 62.52(7) . 3_565 ? 
Na2 P3 Ba2 159.0(2) 3 3_565 ? 
Ca2 P3 Ba2 159.0(2) 3 3_565 ? 
Na2 P3 Ba2 67.13(9) 3_565 3_565 ? 
Ca2 P3 Ba2 67.13(9) 3_565 3_565 ? 
Ca2 P3 Ba2 67.13(9) 3_455 3_565 ? 
Na2 P3 Ba2 67.13(9) 3_455 3_565 ? 
O3 P3 Ba2 116.6(3) 5_665 3 ? 
O3 P3 Ba2 46.0(5) 3 3 ? 
O3 P3 Ba2 132.0(3) 6_565 3 ? 
O6 P3 Ba2 62.52(7) . 3 ? 
Na2 P3 Ba2 67.13(9) 3 3 ? 
Ca2 P3 Ba2 67.13(9) 3 3 ? 
Na2 P3 Ba2 159.0(2) 3_565 3 ? 
Ca2 P3 Ba2 159.0(2) 3_565 3 ? 
Ca2 P3 Ba2 67.13(9) 3_455 3 ? 
Na2 P3 Ba2 67.13(9) 3_455 3 ? 
Ba2 P3 Ba2 100.40(8) 3_565 3 ? 
P2 O1 Na4 149.5(6) 3_554 . ? 
P2 O1 Na12 107.1(5) 3_554 1_545 ? 
Na4 O1 Na12 99.9(4) . 1_545 ? 
P2 O1 Na1 114.0(5) 3_554 1_545 ? 
Na4 O1 Na1 87.8(4) . 1_545 ? 
Na12 O1 Na1 19.1(5) 1_545 1_545 ? 
P2 O1 Ba1 102.8(5) 3_554 . ? 
Na4 O1 Ba1 90.0(5) . . ? 
Na12 O1 Ba1 91.7(4) 1_545 . ? 
Na1 O1 Ba1 106.5(4) 1_545 . ? 
P2 O1 Na3 82.5(5) 3_554 3_554 ? 
Na4 O1 Na3 77.5(4) . 3_554 ? 
Na12 O1 Na3 104.2(4) 1_545 3_554 ? 
Na1 O1 Na3 87.2(4) 1_545 3_554 ? 
Ba1 O1 Na3 161.2(4) . 3_554 ? 
P1 O2 Na4 149.7(8) . . ? 
P1 O2 Na3 111.1(6) . 3_554 ? 
Na4 O2 Na3 90.8(5) . 3_554 ? 
P1 O2 Na1 77.9(6) . . ? 
Na4 O2 Na1 79.9(4) . . ? 
Na3 O2 Na1 94.2(4) 3_554 . ? 
P1 O2 Ba2 106.4(6) . . ? 
Na4 O2 Ba2 89.5(5) . . ? 
Na3 O2 Ba2 99.6(5) 3_554 . ? 
Na1 O2 Ba2 162.7(5) . . ? 
P3 O3 Ca2 100.6(3) 3_554 1_545 ? 
P3 O3 Na2 100.6(3) 3_554 1_545 ? 
Ca2 O3 Na2 0.0(4) 1_545 1_545 ? 
P3 O3 Ba2 110.2(7) 3_554 . ? 
Ca2 O3 Ba2 90.7(3) 1_545 . ? 
Na2 O3 Ba2 90.7(3) 1_545 . ? 
P3 O3 Ba1 144.7(7) 3_554 3 ? 
Ca2 O3 Ba1 94.5(3) 1_545 3 ? 
Na2 O3 Ba1 94.5(3) 1_545 3 ? 
Ba2 O3 Ba1 101.26(17) . 3 ? 
P3 O3 Na2 83.7(3) 3_554 . ? 
Ca2 O3 Na2 172.6(4) 1_545 . ? 
Na2 O3 Na2 172.6(4) 1_545 . ? 
Ba2 O3 Na2 82.0(3) . . ? 
Ba1 O3 Na2 85.3(2) 3 . ? 
P1 O4 Na2 180.000(2) . . ? 
P1 O4 Ba2 93.5(4) . 1_565 ? 
Na2 O4 Ba2 86.5(4) . 1_565 ? 
P1 O4 Ba2 93.5(4) . . ? 
Na2 O4 Ba2 86.5(4) . . ? 
Ba2 O4 Ba2 119.63(8) 1_565 . ? 
P1 O4 Ba2 93.5(4) . 1_665 ? 
Na2 O4 Ba2 86.5(4) . 1_665 ? 
Ba2 O4 Ba2 119.63(8) 1_565 1_665 ? 
Ba2 O4 Ba2 119.63(8) . 1_665 ? 
P2 O5 Na2 180.000(2) . . ? 
P2 O5 Ba1 92.5(4) . 3_565 ? 
Na2 O5 Ba1 87.5(4) . 3_565 ? 
P2 O5 Ba1 92.5(4) . 3 ? 
Na2 O5 Ba1 87.5(4) . 3 ? 
Ba1 O5 Ba1 119.80(7) 3_565 3 ? 
P2 O5 Ba1 92.5(4) . 3_665 ? 
Na2 O5 Ba1 87.5(4) . 3_665 ? 
Ba1 O5 Ba1 119.80(7) 3_565 3_665 ? 
Ba1 O5 Ba1 119.80(7) 3 3_665 ? 
P3 O6 Na3 180.000(3) . . ? 
P3 O6 Ba2 91.6(2) . 3_565 ? 
Na3 O6 Ba2 88.4(2) . 3_565 ? 
P3 O6 Ba2 91.6(2) . 3_665 ? 
Na3 O6 Ba2 88.4(2) . 3_665 ? 
Ba2 O6 Ba2 119.92(2) 3_565 3_665 ? 
P3 O6 Ba2 91.6(2) . 3 ? 
Na3 O6 Ba2 88.4(2) . 3 ? 
Ba2 O6 Ba2 119.92(2) 3_565 3 ? 
Ba2 O6 Ba2 119.92(2) 3_665 3 ? 
